
==== Front
Materials (Basel)
Materials (Basel)
materials
Materials
1996-1944 MDPI 

10.3390/ma13102423
materials-13-02423
Article
Influence of Desulfurization with Fe2O3 on the Reduction of Nickel Converter Slag
Wei Guangsheng 12 Wang Yun 13* Zhu Rong 12 Yang Lingzhi 4* 1 School of Metallurgical and Ecological Engineering, University of Science and Technology Beijing, Beijing 100083, China; danielkhan@example.org (G.W.); danielkhan@example.org (R.Z.)
2 Beijing Key Laboratory of Research Center of Special Melting and Preparation of High-End Metal Materials, University of Science and Technology Beijing, Beijing 100083, China
3 The China ENFI Engineering Co., Ltd., Beijing 100038, China
4 School of Minerals Processing and Bioengineering, Central South University, Changsha 410083, China
* Correspondence: danielkhan@example.org (Y.W.); danielkhan@example.org (L.Y.)
25 5 2020 
5 2020 
13 10 242305 4 2020 19 5 2020 © 2020 by the authors.2020Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).Generally in the nickel converter slag, metals are mainly in the form of sulfides, which are difficult to separate from slag. Although metal oxides in the slag, such as NiO, CoO, and Cu2O, are easily reduced into metal using carbon, the presence of sulfur inhibits the reduction reaction. In this study, the addition of Fe2O3 to nickel converter slag produced desulfurized slag, which enhanced the carbothermal reduction process. Increasing the desulfurization rate promoted the conversion of sulfides into oxides in slag, which significantly increased the activity of NiO, Cu2O, and Fe2O3. However, the residual sulfur content had no significant effect on the activity of FeO and CoO, due to the high initial FeO content and cobalt existing mainly in the form of oxides. The optimum addition of Fe2O3 was 15.0 g per 100 g nickel slag, while the desulfurization ratio was 36.84% and the rates of nikel, cobalt and copper recovery were 95.33%, 77.73%, and 73.83%, respectively.

nickel converter slagdesulfurizationreductionFe2O3metal recovery
==== Body
1. Introduction
The process of oxidizing low-nickel matte using flowing air in a horizontal converter results in a large amount of slag containing nickel, cobalt, copper, and other metals. A subsequent process is used to clean the nickel slag in order to extract some of the nickel, cobalt, and copper [1,2,3]. The molten slag is poured into the melting pool of an electric furnace; then, a matte with high sulfur content is produced by adding coal and pyrite [4,5]. However, the treatment cycle is long and gives poor dilution results of residue copper up to 0.5–1.0% [6,7]. According to previous studies [8], the main components of nickel converter slag is FeO and SiO2, where Ni mainly exists as sulfides and some distributes in fayalite or composite oxides. Cobalt is mainly dispersed in fayalite and most of the copper exists as sulfides [9,10]. Therefore, in the nickel converter slag, the sulfides of Ni and copper result in the loss of Ni and Cu [11,12].

It is of great importance to separate the matte from the slag for the recovery of valuable metals and some key performance parameters determines the separation of matte and slag, including density, viscosity and interfacial tension. Various studies have been carried out to investigate the matte and slag's interfacial tension and density in alloy–slag system [13,14,15,16,17,18,19,20]. For molten slag systems, the density values of FeOx-SiO2-Al2O3 [13], FeOx-SiO2-MgO [13] and FeOx-SiO2-CaO-Al2O3 [14] are in the range of 3.68~3.69 g/cm3, 3.61~3.69 g/cm3 and 2.794~2.836 g/cm3 respectively. For molten matte systems, the density values of Fe-Ni-S [13], Ni-Cu-S [13] and Fe-Cu-Ni-S [15] are in the range of 3.82~5.18 g/cm3, 5.18~5.25 g/cm3 and 3.92~5.59 g/cm3 respectively. For molten metal systems, the density values of Ni-Cu-Fe [16], Fe [17], Ni [17] and Co-Cu-Fe [18] are in the range of 7.1~8.0 g/cm3, 6.905~7.25 g/cm3, 7.60~7.73 g/cm3 and 7.22~7.62 g/cm3 respectively. As for the interfacial tension between molten slag and matte, the values of Fe-Ni-S & FeOx-SiO2-Al2O3, Fe-Ni-S and FeOx-SiO2-MgO are in the range of 0.005~0.180 N/m, 0.026~0.192 N/m [13]. And for that between molten slag and metal, the values of Fe-Ni and CaO-SiO2-Al2O3 is in the range of 0.960~1.670 N/m [19,20]. It can be found that the distribution range of the density of slag is comparatively close to that of the matte while the interfacial tension between matte and slag is particularly small. Hence, the matte can be easily dispersed in the molten slag and it is difficult to separate the matte from the slag. Conversely, it is obvious that the density of the metal with lower sulfur is much larger than that of slag and the value of the interfacial tension between metal and slag is much higher, which indicates that metals are easy to separate from slag using density separation methods. For the nickel converter slag, if the reduction product after desulfurization in the electric furnace is metal rather than matte, a metal containing large amounts of nickel, cobalt, and copper can more easily be separated from the slag. The resulting metal has lower sulfur content than the matte, which is achieved by first removing sulfur and then reducing the metal oxides in the slag.

CaO was used to remove the sulfur for molten metal by forming CaS in the molten metal with low sulfur content [21,22,23]. And with high sulfur content, the sulfur was removed as SO2 with the method of gasification desulfurization [24,25,26]. Li et al. [27] found that high sulfur content of molten iron would cause the generated iron worthless when using the direct smelting reduction method. Huang et al. [28] and Hu et al. [29] studied the effect of the secondary refining on the removal of sulfur from the slag. Li et al. [30] studied the process the smelting oxidation-reduction process of copper slags with air blowing. And results show that the sulfur content can be reduced from 0.52 wt.% to less than 0.01 wt.% with this method. However, it should be noted that blowing air would lead to the peroxidation of the molten slag and as a result, a large amount of reductant would be consumed and the smelting time is increased. Therefore, it is necessary to utilize weak oxidant to remove sulfur firstly in the recovery of valuable metals from the nickel converter slag through oxidation and reduction. The method of Fe2O3 injection was proposed for desulfurization before the reduction of nickel converter slag because Fe2O3 is a weak oxidant and it has an oxidizing effect on slag theoretically. However, few theoretical and experimental studies of the effect of Fe2O3 on the desulfurization of nickel converter slag. What's more, metal oxides such as NiO, CoO, and Cu2O are easily reduced into metals, while sulfur in the slag cannot participate in the reduction reaction [31,32]. For example, NiO is extremely prone to reduction by CO, while Ni3S2 is of great difficulty to reduce, similar to the behavior of Cu2O and Cu2S [33,34,35,36]. The removal of sulfur decreases the ratio of sulfides to oxides, which increases the activity of oxides and promotes the reduction reaction and formation of metals.

In this study, theoretical analysis and tubular furnace experiments were carried out to investigate the effect of desulfurization with Fe2O3 on the smelting oxidation-reduction process of nickel converter slag. The Fe2O3 was used to remove the sulfur from the molten slag with sulfur content being 1.53 wt.%. And then carbon was applied to deal with the desulfurized slags with different sulfur contents. The thermodynamic software program FactSage 7.0 was used to simulate the process of slag oxidation, and the simulated data were compared with experimental results. In addition, the desulfurization rate and recovery of valuable metal was studied.

2. Thermal State Experiment
2.1. Materials
In this study, the nickel converter slag from Jilin Jien Nickel Industry smelter factory (Jilin, China) was adopted. And the method of chemical analysis was applied to test the raw materials and slag and metals from the experiment. As reported by previous studies [8,9,10,11,37], nickel mainly exists as sulfides and some distributes in fayalite or composite oxides, cobalt is mainly dispersed in fayalite and copper mainly exists as sulfides. The elemental distribution of nickel, cobalt, and iron in nickel converter slag is dispersive and uniform. In this study, the remaining moisture was removed by drying the sample slag for 6 h at 110 °C. The slag was processed into powder and the ratio of powder that being less than 100 mesh is larger than 95%. Table 1 lists the chemical composition of nickel converter slag. The chemical compositions of the nickel converter slag are 3.51 wt.% Ni, 0.60 wt.% Co, 0.92 wt.% Cu, 1.53 wt.% S, 43.2 wt.% Total Fe, 52.8 wt.% FeO, 29.2 wt.% SiO2, 0.11 wt.% CaO, 0.83 wt.% MgO, and 0.48 wt.% Al2O3; the ferric oxide (Fe2O3 > 99.0 wt.%) was applied as the oxidizer; and carbon powder (C > 99.85 wt.%) was applied as the reducing agent.

2.2. Experiments
Figure 1 presents the thermal experiment flat platform used in this study, including a tubular furnace (Zhongkebeiyi, Beijing, China) with Ar protective gas. The sample was placed in an alumina crucible (φ40 mm × 90 mm), and held in an alumina safety crucible (φ60 mm × 150 mm) to protect the furnace tube from inner crucible failure. The furnace temperature was increased to 1000 °C at a rate of 10 °C/min. Then, the crucible containing the sample was placed in the tubular furnace at 1000 °C. The furnace was resealed and the furnace temperature was further increased from 1000 to 1300 °C at a rate of 5 °C/min; then the temperature was maintained at 1300 °C for desulfurization or reduction. The slag and metal obtained from the experiments were analyzed in Testing Center of University of Science and Technology Beijing (USTB).

Table 1 shows the experimental schemes for the desulphurization of initial nickel converter slag with Fe2O3. The Fe2O3 (0–40.0 g) and the nickel converter slag (100.0 g) were mixed in the desired ratios and these mixtures were held at 1300 °C for 30 min. Then, the molten slag was cooled in flowing Ar. Half of the cooled desulfurized slag was applied in the subsequent reduction experiments, while the remainder was used for analysis by a SPECTRO X-ray Fluorescence Spectrometer, SPECTRO Analytical Instruments, Kleve, Germany.

Table 2 shows the experimental schemes for the reduction of the desulfurized slag with carbon powder. In this study, the carbon powder was added with the C/O ratio danielkhan@example.org. The desulfurized slag (~50–70 g) and the carbon powder were mixed, and the mixture was heat treated at 1300 °C for 60 min. After reduction and separation, the sample was cooled in flowing argon. The metal formed in the reduction experiments were sent for analysis.

The FactSage 7.0 thermodynamics software (7.0, FactSage, GTT-Technologies, Herzogenrath, Germany) was used to characterize the chemical equilibrium of the reactions during the desulfurization process, and the activities of FeO, Fe2O3, NiO, CoO, and Cu2O during this process were calculated. According to previous research [37], the ratios of Ni, Co, and Cu existing as sulfide were 51.64%, 15.33%, and 90.08%, respectively. It was assumed that Equation (1) the ratios of Ni, Co, and Cu existing as sulfide were, respectively, 50%, 15%, and 90% and Equation (2) all other sulfur in the slag existed as FeS. The input data used for simulations with the Equilib module of FactSage were 2.23 wt.% NiO, 2.39 wt.% Ni3S2, 0.65 wt.% CoO, 0.14 wt.% CoS, 0.10 wt.% Cu2O, 1.04 wt.% Cu2S, 3.00 wt.% Fe2O3, 51.40 wt.% FeO, 1.76 wt.% FeS, 29.20 wt.% SiO2, and 8.09 wt.% Al2O3 (The total slag weight was 100 g, and other substances in the slag were supplemented using Al2O3).

3. Results and Discussions
3.1. Liquidus Temperature of Desulfurized Slag
In the nickel converter slag, the total content of FeOx and SiO2 was larger than 80% and the liquidus temperature of slag was determined using FeO-Fe2O3-SiO2 phase diagram [38,39,40,41]. Although the increase in the slag liquidus temperature had almost no influence on the desulfurization and reduction progress, it is helpful to separate the metal from the slag with the slag with a lower liquidus temperature [42]. According to the previous study [37], it can be known that the addition of Fe2O3 influences the liquidus temperature of the slag significantly. The liquidus temperature of slag can be reduced when the Fe2O3 addition being less than 6 wt.% and that would be increased when the Fe2O3 addition in the range of 6–40 wt.%. According to the composition of total Fe and FeO in desulfurized slag in Table 2, the content of FeO, Fe2O3 and SiO2 can be calculated. The composition of the desulfurized slag in the ternary phase diagram of FeO-Fe2O3-SiO2 is shown in Figure 2. With the addition of Fe2O3, the composition of slag moves towards the region with high liquidus temperature.

3.2. Equilibrium of Sulfide and Oxide in Slag
Although Fe2O3 has weaker oxidizing performance than O2, the added Fe2O3 can react with the sulfides (Ni3S2, CoS, Cu2S, and FeS) in the slag. The reactions are as follows: 7Fe2O3 + Ni3S2 = 14FeO + 3NiO + 2SO2 (g)(1)  
 (2) ΔGNi=ΔGNiθ+RTlnaFeO14·aNiO3·(pSO2/pθ)2aFe2O37·aNi3S2 
 3Fe2O3 + CoS = 6FeO + CoO + SO2 (g)(3)  
 (4) ΔGCo=ΔGCoθ+RTlnaFeO6·aCoO·(pSO2/pθ)aFe2O33·aCoS 
 3Fe2O3 + Cu2S = 6FeO + Cu2O + SO2 (g)(5)  
 (6) ΔGCu=ΔGCuθ+RTlnaFeO6·aCu2O·(pSO2/pθ)aFe2O33·aCu2S 
 3Fe2O3 + FeS = 7FeO + SO2 (g)(7)  
 (8) ΔGFe=ΔGFeθ+RTlnaFeO7·(pSO2/pθ)aFe2O33·aFeS 
where ΔGM (M = Ni, Co, Cu, and Fe) is the Gibbs free energy (J/mol) of the chemical reactions, ΔGMθ is the Gibbs free energy in the standard state, R = 8.314 J/(mol·K) is the universal gas constant, T is temperature (K), aN is the activity of N (N = Fe2O3, FeO, NiO, CoO, Cu2O, FeS, Ni3S2, CoS, and Cu2S) in the slag, pSO2 is the partial pressure of gaseous SO2 (Pa), and pθ is the standard atmospheric pressure, 101325 Pa. When the desulfurization reaction reaches equilibrium, ΔG = 0. The ratio of the sulfides to oxides in the slag changed gradually during oxidation. At constant temperature conditions (1300 °C), the distribution ratio depends on the composition of the melting slag (NiO, FeO, and Fe2O3 contents) and the SO2 partial pressure (pSO2). Based on the above reactions, it can be found that a high Fe3+/Fe2+ ratio, resulting in a low aFeO2aFe2O3 ratio and low pSO2, are beneficial for converting sulfides to oxides. This agreed with previous reports [11,15]. The ratio of Fe3+/Fe2+ is mainly influenced by the amount of added Fe2O3, while pSO2 is mainly influenced by the rate of SO2 release during the reaction. Figure 3 shows that the ratio of Fe3+/Fe2+ in the slag measured experimentally increased with increasing Fe2O3 content, consistent with the theoretical calculations. In this paper, the equilibrium value of sulfur in slag has a balance relationship with SO2 concentration in the gas phase. When Fe2O3 was used for desulfurization reaction in the tubular furnace, the release rate of SO2 is different under different conditions, but the flow rate of argon is not constant all the time, which will cause a great difference in SO2 concentration in the gas phase. Therefore, results with different SO2 partial pressure were calculated by Factsage calculation as shown in Figure 3. What's more, When more Fe2O3 was added (30 g, 40 g), more Fe2O3 will not participate in the reaction of sulfide oxidation, and the utilization rate of oxidant is low, so that the Fe3+ remaining in slag is higher, causing the curve to deviate from the calculated value of Factsage calculation.

3.3. Desulphurization Rate
In order to compare the influence of Fe2O3 addition on sulfur removal, the desulfurization rate was defined as: (9) φ=1−m·w(S)m0·w0(S)×100% 
where φ is the desulfurization rate (%), m is the mass of the slag after the desulfurization (g), m0 is the mass of initial nickel converter slag (g), w(S) is the mass fraction of sulfur in the desulfurized slag (%), and w0(S) is the mass fraction of sulfur in the initial nickel converter slag (%).

Figure 4 shows the relationship between the added Fe2O3 and the desulfurization rate for both experimental and theoretical results. When a small amount of Fe2O3 was added (0–5 wt.%), the desulfurization rate was relatively low after reaction. In this case, the initial Fe2O3 content in the slag was low, and most of added Fe2O3 was dissolved into the slag instead of participating in the desulfurization reaction. When 10–20 wt.% Fe2O3 was added, the slag was strongly oxidized, where the sulfur in the slag was oxidized to SO2. Hence, the desulfurization rate increased significantly with the addition of Fe2O3, as shown in Figure 4. With further addition of Fe2O3 (20–40 wt.%), the rate of increase of the desulfurization rate decreased. Under these conditions, the sample could not reach equilibrium within the limited time of the experiment due to the high viscosity of the slag. Therefore, the desulfurization rate increased slowly and inadequate contact between S2− and Fe2O3 in the slag was the main limiting factor for the desulfurization reaction [43]. In addition, the SO2 concentration of the product in the reaction process will affect the sulfur content of the equilibrium slag, while the SO2 concentration in the gas phase will be different due to the different SO2 release rate in the oxidation desulfurization reaction during the experiment process, which may affect the different desulfurization process. The Factsage calculation can quantify and compare the equilibrium value under different SO2 partial pressure with the test results.

3.4. Activity of Metal Oxide in Slag
Ni, Co, and Cu mainly existed as NiO, CoO, Cu2O, Ni3S2, CoS, and Cu2S in the slag. The gaseous products of oxides reduced by carbon are mainly CO, while the gaseous products of sulfide reduction are mainly CS2 [38]. According to our previous study [37], the Standard Gibbs free energy of relative reactions have been obtianed from thermodynamic modeling using FactSage. Considering the change in the Gibbs free energy, carbon reacts most readily, first with metal oxides and then with sulfides, in the order of Cu2O, NiO, CoO, FeO, Fe2SiO4, CoS, Ni3S2, FeS, and Cu2S. The ability to oxidize the slag has an equilibrium relationship with the sulfur content in the desulfurized slag, which further influences the ratio of metal sulfides to oxides. According to our previous study [37], the predominant reactions were the reduction of metal oxides by carbon and the increases in the activities of FeO, Fe2O3, NiO, CoO, and Cu2O in the slag could promote the reduction reaction.

As shown in Figure 5a, the activities of FeO, Fe2O3, NiO, CoO, and Cu2O in desulfurized slag were exported from FactSage to analyze the influence of desulfurization rate on the activity of metal oxide in the desulfurized slag. With the addition of Fe2O3, the sulfur content decreased and the activities of FeO, Fe2O3, NiO, and Cu2O increased, while the activity of CoO was almost not affected by the increase of Fe2O3 addition.

In order to compare the relative changes in activity, the activity of the oxides changes with the amount of Fe2O3 addition was defined as: α = (a − a1)/a1 × 100%(10)  
where a is the activity of oxides in Experiment No. 1–7; a1 is the activity of the oxides after desulfurization in Experiment No. 1.

With the addition of Fe2O3, the increase of activity in Cu2O, NiO, and Fe2O3 were significantly, while the increase of activity in FeO and CoO were not. Although Fe2O3 was added, the most notable increase in activity was for Cu2O, rather than Fe2O3 or FeO, according to Figure 5b. The added Fe2O3 reacted with sulfides, such as Ni3S2, CoS, and Cu2S, where the sulfur was removed in the form of SO2. After sulfur removal from the slag, sulfides in the slag were converted into oxides, increasing the amount (and activity) of metal oxides in the slag. According to the analysis of the existing forms of nickel, cobalt, and copper in nickel slag [44], copper exists mainly in the form of sulfide, which makes sulfur removal have the most significant effect on copper oxide and sulfide in the slag. However, cobalt mainly exists in the form of oxide, and its activity was barely affected by sulfur in the slag. Although most of the added Fe2O3 was oxidized to FeO, the Fe2+ in the slag increased, while Fe3+/Fe2+ increased simultaneously. Because of the high initial FeO content, the increase in Fe3+ fraction was larger, i.e., ΔFe3+/Fe3+ was greater than ΔFe2+/Fe2+ (ΔFe3+ and ΔFe2+ are the increase in the Fe3+ and Fe2+ ion concentrations in the slag, respectively). This resulted in a larger rate of change in activity for Fe2O3 than FeO, as shown in Figure 5b.

3.5. Recovery of Nickel, Cobalt, and Copper
Figure 6 shows the Ni, Co and Cu recovery rates change with different addition of Fe2O3. With the Fe2O3 addition increased in the range of 0–15.0 g, the metals recovery rates increased. However, with the addition of Fe2O3 further increasing from 15.0 to 40.0 g, the metals recovery rate declined sharply. According to the phase diagram of FeO-Fe2O3-SiO2, the slag will melt very well at 1500 °C, while the phase diagram of Fe-Ni-Co-Cu-S shows that the decrease of sulfur content will make the liquidus temperature of metal increase significantly [45,46,47,48,49]. With the increase of Fe2O3 addition, the sulfur content in metal decreased, causing the high liquidus temperature of metal and poor separation of metal from slag. Therefore, although the removal of sulfur from slag promotes the reduction of oxides, the liquidus temperature of metal obtained increases simultaneously. The optimum addition of Fe2O3 was 15.0 g, while the desulfurization rate was 36.82% and the Ni, Co and Cu recovery rate were 95.33%, 77.73%, and 73.83%, respectively.

4. Conclusions
The Fe2O3 was used to remove sulfur firstly in the recovery of Ni, Co and Cu from the nickel converter slag as a weak oxidant due to the peroxidation of the molten slag with blowing air in the smelting oxidation-reduction process of nickel converter slag. The theoretical analysis and tubular furnace experiments were carried out to investigate the effect of desulfurization with Fe2O3 on the production process. The main conclusions are as following:(1) the liquidus temperature decreased with the addition of Fe2O3 being in the range of 0–6 wt.%. however, the liquidus temperature began to increase for a Fe2O3 content of 6–40 wt.%. In addition, the desulfurization rate increased with the addition of Fe2O3, where the growth was the most significant for Fe2O3 contents of 5–20%.

(2) According to the FactSage calculations, a higher desulfurization rate of the slag promoted conversion of sulfides into oxides, which significantly increased the activities of Cu2O, NiO, and Fe2O3 in the slag. However, activity of CoO and FeO was not significantly affected.

(3) Although the removal of sulfur from slag promotes the carbothermic reduction of oxides, the liquidus temperature of metal obtained increases simultaneously. The optimum addition of Fe2O3 was 15.0 g, while the desulfurization rate was 36.82% and the metal recovery rate of Ni, Co, and Cu were 95.33%, 77.73%, and 73.83%, respectively.



Author Contributions
Conceptualization, G.W. and Y.W.; Methodology, G.W. and L.Y.; software, Y.W.; Validation, Y.W. and L.Y.; Formal analysis, G.W. and Y.W.; Investigation, G.W. and Y.W.; Resources, R.Z.; Data curation, L.Y. and R.Z.; Writing—original draft preparation, G.W. and Y.W.; Writing—review and editing, G.W. and Y.W.; Visualization, L.Y.; Supervision, L.Y. and R.Z.; Project administration, G.W. and R.Z.; Funding acquisition, G.W. All authors have read and agreed to the published version of the manuscript.

Funding
The authors would like to express their thanks for the support by the Fundamental Research Funds for the Central Universities (FRF-TP-19-031A1), the China Post Postdoctoral Science Foundation (2019M660459), and the National Nature Science Foundation of China (NO.51804345, NO.51734003 & NO.51674021).

Conflicts of Interest
The authors declare no conflicts of interest.

Figure 1 Schematic of the experimental equipment.

Figure 2 Phase diagram of slag: desulphurization slag composition in the ternary phase diagram of FeO-Fe2O3-SiO2 (obtained from FactSage).

Figure 3 Variation of slag oxidation (Fe3+/Fe2+) with Fe2O3 addition.

Figure 4 Effect of Fe2O3 addition on desulfurization rate.

Figure 5 Addition of Fe2O3 versus (a) activity of oxides, and (b) activity change rate of oxides.

Figure 6 Addition of Fe2O3 versus metals recovery rate.

materials-13-02423-t001_Table 1Table 1 Experimental schemes for the desulphurization of initial nickel converter slag with Fe2O3.

No.	Initial Slag (g)	Fe2O3 (g)	Final Slag (g)	Composition of Slag (wt.%)	
Fe	FeO	Ni	Co	Cu	S	Al2O3	
1	100.0	0.0	99.4	43.3	52.82	3.52	0.60	0.94	1.50	1.26	
2	100.0	5.0	103.6	44.7	53.91	3.36	0.57	0.90	1.41	1.52	
3	100.0	10.0	108.0	46.1	53.21	3.22	0.55	0.86	1.03	1.83	
4	100.0	15.0	112.4	47.4	53.79	3.10	0.53	0.83	0.86	1.57	
5	100.0	20.0	116.9	48.4	54.21	2.97	0.51	0.80	0.59	1.76	
6	100.0	30.0	126.5	50.3	54.48	2.75	0.47	0.74	0.40	1.35	
7 *	100.0	40.0	135.6	51.9	55.19	2.57	0.44	0.69	0.33	1.41	
* With the poor separation of slag and alloy in Experiment No. 7, the alloy contains lots of slag.

materials-13-02423-t002_Table 2Table 2 Experimental schemes for the reduction of the desulfurized slag with carbon powder.

No.	Initial Slag (g)	Carbon Powder
(C/O = 0.2) (g)	Mass of Alloy (g)	Composition of Alloy (wt.%)	
Ni	Co	Cu	S	
1	49.7	1.04	6.42	25.25	3.49	5.14	2.92	
2	51.8	1.11	6.39	25.62	3.45	5.13	2.55	
3	54.0	1.21	6.94	23.60	3.29	4.87	1.58	
4	56.2	1.30	7.19	23.10	3.22	4.79	1.20	
5	58.5	1.38	6.23	22.01	2.75	4.63	0.77	
6	63.2	1.56	4.65	20.11	3.12	4.33	0.45	
7 *	67.8	1.73	−	−	−	−	−	
* With the poor separation of slag and alloy in Experiment No. 7, the alloy contains lots of slag.
==== Refs
References
1. Diaz C.M.  Landolt C.A.  Vahed A.  Warner A.E.M.  Taylor J.C.   A Review of Nickel Pyrometallurgical Operations JOM 1988 40 28 33 10.1007/BF03258548 
2. Liu X.M.  Gao S.L.  Jie L.I.  Kou J.  Sun C.B.   Process mineralogy of jinchuan nickel slag in a settlement furnace Chin. J. Eng. 2017 39 349 078-50-35034/j.issn2095-9389.2017.03.005 (In Chinese) 
3. Zhang H.  Dong J.  Xiong H.  Wang Z.  Lu Y.   Investigation on cooperative desulfurization efficiency for bearing carbon stainless steel dust briquettes chromium and nickel recovery process J. Alloys Compd. 2017 699 408 078-50-3503/j.jallcom.2016.12.362 
4. Yu Z.J.  Feng Q.M.  Ou L.M.  Lu Y.P.  Zhang G.F.   Recovery of cobalt, nickel and copper from nickel converter slag by reduction-sulfurization process Min. Metall. Eng. 2006 26 49 55 10.3969/j.issn.0253-6099.2006.01.014 (In Chinese) 
5. Yu D.  Chattopadhyay K.   Enhancement of the nickel converter slag-cleaning operation with the addition of spent potlining Int. J. Miner. Metall. Mater. 2018 25 881 078-50-3503/s12613-018-1637-0 
6. Coman V.  Robotin B.  Ilea P.   Nickel recovery/removal from industrial wastes: A review Resour. Conserv. Recycl. 2013 73 229 078-50-3503/j.resconrec.2013.01.019 
7. Li X.M.  Shen M.  Wang C.  Cui Y.  Zhao J.   Current situation and development of comprehensive utilization of nickel slag Mater. Rep. 2017 31 100 078-50-35036/j.issn.1005-023X.2017.05.016 (In Chinese) 
8. Yang T.  Yao X.  Zhang Z.   Geopolymer prepared with high-magnesium nickel slag: Characterization of properties and microstructure Constr. Build. Mater. 2016 59 188 078-50-3503/j.conbuildmat.2014.01.038 
9. Cao Z.M.  Sun G.S.  Richter K.  Qiao Z.Y.   Microstructure and metal distribution in jinchuan nickel smelting slag J. Univ. Sci. Technol. Beijing 2001 23 316 078-50-3503/j.issn:1001-053X.2001.04.008 (In Chinese) 
10. Mikhail S.A.  Webster A.H.   Recovery of nickel, cobalt and copper from industrial slag extraction into iron sulphide matte Can. Metall. Q. 1992 31 269 078-50-3503/cmq.1930.078-50-3503 
11. Nagamori M.   Metal loss to slag: Part II. oxidic dissolution of nickel in fayalite slag and thermodynamics of continuous converting of nickel-copper matte Metall. Trans. 1974 5 539 078-50-3503/BF02644647 
12. Ruşen A.  Geveci A.  Topkaya Y.A.  Derin B.   Investigation of effect of colemanite addition on copper losses in matte smelting slag Can. Metall. Q. 2013 51 157 2078-50-3503/1879139512Y.0000000005 
13. Ip S.W.  Toguri J.M.   Surface and interfacial tension of the Ni-Fe-S, Ni-Cu-S, and fayalite slag systems Metall. Trans. B 1993 24 657 078-50-3503/BF02673181 
14. Sun H.  Nakashima K.  Mori K.   Influence of slag composition on slag-iron interfacial tension ISIJ Int. 2006 46 407 078-50-3503/isijinternational.46.407 
15. Mungall J.E.  Su S.   Interfacial tension between magmatic sulfide and silicate liquids: Constraints on kinetics of sulfide liquation and sulfide migration through silicate rocks Earth Planet. Sci. Lett. 2005 234 135 078-50-3503/j.epsl.2005.02.035 
16. Brillo J.  Egry I.  Matsushita T.   Density and Surface Tension of Liquid Ternary Ni–Cu–Fe Alloys Int. J. Thermophys. 2078-50-3503 1078-50-3503/s10765-006-0121-7 
17. Sharan A.  Nagasaka T.  Cramb A.W.   Densities of liquid Fe-Ni and Fe-Cr alloys Metall. Mater. Trans. B 1994 25 939 942 10.1007/BF02662777 
18. Brillo J.  Egry I.   Density and surface tension of electromagnetically levitated Cu-Co-Fe alloys Int. J. Thermophys. 2078-50-3503 1078-50-3503/s10765-007-0209-8 
19. Sharan A.  Cramb A.W.   Interfacial Tensions of Liquid Fe-Ni Alloys and Stainless Steels in Contact with CaO-SiO2 -Al2 O3 -Based Slags at 1550 °C Metall. Mater. Trans. B 1995 26 87 94 10.1007/BF02648981 
20. Sun H.  Yoneda N.  Nakashima K.  Mori K.   Interfacial Tensions between CaO-SiO2 -Al2 O3  slag and Fe-O-S, Fe-Si, Fe-Al, Fe-C, Fe-Cr or Fe-Ni Alloys Tetsu-to-Hagané 1997 83 1 6 10.2355/tetsutohagane1955.83.1_1 
21. Turkdogan E.T.  Martonik L.J.   Sulfur Solubility in Iron-Carbon Melts Coexistent with Solid CaO and CaS Trans. Iron Steel Inst. Jpn. 1983 23 1038 1078-50-3503/isijinternational1966.23.1038 
22. Lindström D.  Du S.   Kinetic Study on Desulfurization of Hot Metal Using CaO and CaC2  Metall. Mater. Trans. B 2015 46 83 92 10.1007/s11663-014-0195-8 
23. Hao X.  Wang X.  Wang W.   Study on Desulfurization Ability of CaO-Al2 O3 -SiO2  and CaO–CaF2  Slags at 1600 °C Steel Res. Int. 2078-50-3503 1078-50-3503/srin.201400401 
24. Long H.M.  Zhang X.Y.  Li J.X.  Wang P.  Meng Q.M.  Gao Z.F.  Chun T.J.  Wu X.J.   Study on Emission Characteristics of SO2  and Feasibility of Desulfurization in Iron Ore Sintering Process Chin. J. Process Eng. 2015 15 230 235 (In Chinese) 
25. Henao H.M.  Itagaki K.   Phase equilibrium and distribution of minor elements between Ni-S melt and Al2 O3 -CaO-MgO Slag at 1873K Metall. Mater. Trans. B 2078-50-3503 1078-50-3503/s11663-004-0060-2 
26. Fukunaka Y.  Nishikawa K.  Sohn H.S.  Asaki Z.   Desulfurization kinetics of molten copper by gas bubbling Metall. Trans. B 1991 22 5 11 10.1007/BF02672520 
27. Li L.  Hu J.  Wang H.   Study on Smelting Reduction Ironmaking of Copper Slag Chin. J. Process Eng. 2011 11 65 71 (In Chinese) 
28. Cheng H.  Ren T.   Deep Desulfurization of Hot Metal Development Trend Iron Steel 2001 36 17 19 (In Chinese) 
29. Hu C.  Zhang C.  Han X.   Sulfur Flow Analysis for New Generation Steel Manufacturing Process J. Iron Steel Res. Int. 2008 15 15 18 10.1016/S1006-706X(08)60136-3 
30. Li L.  Hu J.H.  Wang H.   Smelting oxidation desulfurization of copper slags J. Iron Steel Res. Int. 2012 19 14 20 10.1016/S1006-706X(13)60026-6 
31. Nagamori M.  Yazawa A.   Thermodynamic observations of the molten FeS-FeO system and its vicinity at 1473K Metall. Mater. Trans. B 2001 32 831 078-50-3503/s11663-001-0070-2 
32. Nagamori M.  Yazawa A.   The Quaternary Gibbs-Duhem Integration for Molten Cu-Fe-S-O Mattes at 1473 K Can. Metall. Q. 2002 41 175 078-50-3503/cmq.230.255.87.135 
33. Garcíalabiano F.  Diego L.F.D.  Gayán P.  Adánez J.  Abad A.  Dueso C.   Effect of Fuel Gas Composition in Chemical-Looping Combustion with Ni-Based Oxygen Carriers. 1. Fate of Sulfur Ind. Eng. Chem. Res. 2078-50-3503 2078-50-3503/ie801332z 
34. Wiheeb A.D.  Shamsudin I.K.  Ahmad M.A.  Murat M.N.  Kim J.  Othman M.R.   Present technologies for hydrogen sulfide removal from gaseous mixtures Rev. Chem. Eng. 2013 29 449 078-50-3503/revce-2013-0017 
35. Wang B.  Yan R.  Dong H.L.  Liang D.T.  Zheng Y.  Zhao H.  Zheng C.G.   Thermodynamic Investigation of Carbon Deposition and Sulfur Evolution in Chemical Looping Combustion with Syngas Energy Fuel 2078-50-3503 1078-50-3503/ef7005673 
36. Utigard T.A.  Wu M.  Plascencia G.  Marin T.   Reduction kinetics of Goro nickel oxide using hydrogen Chem. Eng. Sci. 2078-50-3503 2078-50-3503/j.ces.2004.11.024 
37. Wang Y.  Zhu R.  Chen Q.  Wei G.  Hu S.  Guo Y.   Recovery of Fe, Ni, Co, and Cu from Nickel Converter Slag through Oxidation and Reduction ISIJ Int. 2078-50-3503 2078-50-3503/isijinternational.ISIJINT-2018-533 
38. Yu Z.   The Study of Theory and Technology of Recovery of Co, Ni and Cu from Nickel Converter Slag Ph.D. Thesis Central South University Changsha, China 2007 
39. Grutzeck M.W.  Muan A.   Liquid–Solid Equilibria in the System FeO–NiO–Fe2 O3 –SiO2  J. Am. Ceram. Soc. 2078-50-3503 1078-50-3503/j.608-498-2793.tb04192.x 
40. Muan A.   Phase Equilibrium Relationships at Liquidus Temperatures in the System FeO–Fe2 O3 –Al2 O3 –SiO2  J. Am. Ceram. Soc. 1957 40 420 078-50-3503/j.608-498-2793.tb12566.x 
41. Jak E.  Hayes P.  Pelton A.  Decterov S.   Thermodynamic optimisation of the FeO-Fe2 O3 -SiO2  (Fe-O-Si) system with FactSage Int. J. Mater. Res. 2007 98 847 078-50-3503/146.101541 
42. Zhu B.X.  Guo W.  Xin J.  Shen F.M.   Melting Separation of Ore-Coal Composite Pellet at Low Temperature J. Northeast. Univ. (Nat. Sci.) 2012 33 537 541 (In Chinese) 
43. Hu X.L.  Chen W.M.  Xie Q.L.   Desulfuration of high sulfur bauxite by oxidation roasting J. Cent. South Univ. (Sci. Technol.) 2010 41 852 858 (In Chinese) 
44. Wang K.  Tian X.  Zhao H.   Sulfur behavior in chemical-looping combustion using a copper ore oxygen carrier Appl. Energy 2016 166 84 95 10.1016/j.apenergy.2016.01.011 
45. Jacob K.T.  Rao D.B.  Nelson H.G.   Phase relations in the Fe-Ni-Cr-S system and the sulfidation of an austenitic stainless steel Oxid. Met. 1979 13 25 55 10.1007/BF00715869 
46. Howald R.A.   The thermodynamics of tetrataenite and awaruite: A review of the Fe-Ni phase diagram Metall. Mater. Trans. A 2078-50-3503 1078-50-3503/s11661-003-0142-9 
47. Sinyakova E.F.   The section of the Fe–Ni–S phase diagram constructed by directional crystallization and thermal analysis J. Therm. Anal. Calorim. 2013 111 71 76 10.1007/s10973-011-2181-6 
48. Starykh R.V.  Sineva S.I.   Study of the liquidus and solidus surfaces of the quaternary Fe-Ni-Cu-S system: V. Refinement and addition of the data on the ternary Fe-Ni-S and Fe-Ni-Cu phase diagrams Russ. Metall. (Met.) 2012 2012 189 078-50-3503/S0036029512030135 
49. Sellamuthu R.  Goldstein J.I.   Measurement and analysis of distribution coefficients in Fe-Ni alloys containing S and/or P: Part II. KIr , KGe , and KCu  Metall. Trans. A 1985 16 1871 1078-50-3503/BF02670374


{'source': 'PubMedDataset'}